#------------------------------------------------------------------------------
#$Date: 2024-05-02 12:48:35 +0200 (Thu 02 de May de 2024) $
#$Revision: 291455 $
#$URL: svn://www.crystallography.net/cod/cif/9/00/61/9006158.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9006158
loop_
_publ_author_name
'Yang, H.'
'Ghose, S.'
'Hatch, D. M.'
_publ_section_title
;
 Ferroelastic phase transition in cryolite, Na3AlF6, a mixed
 fluoride perovskite: high temperature single crystal X-ray
 diffraction study and symmetry analysis of the transition mechanism
 Sample: T = 373 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              528
_journal_page_last               544
_journal_volume                  19
_journal_year                    1993
_chemical_formula_sum            'Al F6 Na3'
_chemical_name_mineral           Cryolite
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.155
_cell_angle_gamma                90
_cell_length_a                   5.4306
_cell_length_b                   5.6069
_cell_length_c                   7.7944
_cell_formula_units_Z            2
_cell_volume                     237.330
_database_code_amcsd             0007740
_diffrn_ambient_temperature      373
_exptl_crystal_density_diffrn    2.938
_cod_original_formula_sum        'Al Na3 F6'
_cod_database_code               9006158
loop_
_space_group_symop_operation_xyz
x,y,z
1/2+x,1/2-y,1/2+z
1/2-x,1/2+y,1/2-z
-x,-y,-z
loop_
_atom_site_aniso_label
_atom_site_aniso_U_11
_atom_site_aniso_U_22
_atom_site_aniso_U_33
_atom_site_aniso_U_12
_atom_site_aniso_U_13
_atom_site_aniso_U_23
Al 0.01863 0.01687 0.03041 0.00011 0.00094 -0.00013
Na1 0.02882 0.02733 0.04838 -0.00433 -0.00028 0.00487
Na2 0.03983 0.03590 0.08562 -0.00740 0.00167 0.00080
F1 0.04050 0.04009 0.03749 0.00049 -0.00791 -0.00418
F2 0.03025 0.03177 0.08211 -0.01415 0.00817 -0.00055
F3 0.03203 0.02840 0.09212 -0.00924 0.00169 0.01337
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
Al 0.00000 0.00000 0.00000
Na1 0.00000 0.00000 0.50000
Na2 -0.01210 0.44920 0.25260
F1 0.10160 0.04420 0.21880
F2 0.22780 0.32670 0.54500
F3 0.16220 0.26870 0.93830
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0007740
